Discussion Chain ID: 115646
================================================================================

User asked: Why isn't 'chemically-strengthened glass' made with potassium carbonate to begin with?

Instead of making potassium-strengthened glass by creating ordinary soda-lime glass first, then replacing the sodium atoms/ions with potassium by putting the glass in a bath/solution of potassium nitrate, why not replace the 'soda' (sodium carbonate) in the initial process(es) with potassium carbonate?

Discussion:
Comment: Related: https://chemistry.stackexchange.com/q/77249/23561
Comment: @A.K. That question (and your answer to it) is actually much more interesting than this one.

Answer 1 (46 votes):
The potassium is not added first because the potassium does not intrinsically make stronger glass, it is the substitution of a larger ion for a smaller one at the surface that does. To understand why ion exchange strengthens glass, you have to understand why the ion exchange makes the glass harder. The process of ion exchange hardening is done at a temperature that allows ion diffusion, but disallows a reconfiguration of the glass structure or relaxation of bonds (i.e. below $T_{g}$, the glass transition temperature). When sodium atoms are replaced by potassium in glass, the potassium ions occupy a site that is sized for sodium. This substitution of ions creates a compressive force in the sites where it occurs. Since the process is diffusive, the compressive force is produced on the surface of the glass and the interior is put in tension. The compressive force at the surface causes any surface defects, namely scratches, to be in compression. These surface defects being in compression prevents their ability to grow or cause failure of the glass, thus strengthening the glass. If you make a glass with potassium, you have potassium ions occupying potassium sites, thus no strengthening occurs. Thus the only way to chemically harden the glass is to substitute larger ions into the glass. > Preemptive Question: What about internal defects causing failure? Gorilla Glass is made via the fusion draw process where molten glass flow over two sides of a platinum trough and meets at the bottom to be rejoined. This process prevents many internal defects to the point that they are very rare and quality control can remove the few pieces with defects that are made.

Discussion on this answer:
Comment: Interesting, is there a way you could make softer glass by replacing potassium with sodium instead? I'm not sure what use that would have, but is it chemically possible?
Comment: Or would that actually also make the glass stronger by adding different kind of stress?
Comment: @KevinWells It would not.
Comment: Do you mean it wouldn't make it stronger or that it would not be possible?
Comment: @KevinWells potassium does not cause stress by being in the glass as any stresses present will relax above the annealing (or melting) temperature. It is only by ion substitution that strengthening will occur.
Comment: But just to be clear on the question here since the answer given *seems to be talking about total substitution of K for Na*:- If this kind of glass needs x wt% substitution of K ions for Na then why not add a suitable amount of the K ions (or some oxide or carbonate of them) into the mix before melting ? Is there some chemical, structural, vitrification or other reason why GG glass can't be processed directly in this way rather than by a secondary post-melting process to infuse the K ions ?
Comment: @Trunk I don't understand, is this not in the answer?
Comment: *If you make a glass with potassium, you have potassium ions occupying potassium sites, thus no strengthening occurs.* This doesn't make much sense to me, an ex-materials scientist. If you mean to say that intimately mixing crushed solid $K_2O$ and $Na_2O$ and melting them together will simply produce a 2 phase oxide mixture on vitrification, then it's a poor way of saying it. There can't be "potassium sites" unless there is a putative phase based on a definite concentration of potassium ions after melting and solidifying.
Comment: The answer by DrMoishe Pippik (see below) makes much more sense. He's *clearly* saying that the diffusion process results in **only a surface layer of the glass** being infiltrated by potassium ions and this produces a compressive stress within that depth which naturally increases the tensile load needed to cause fracture in it. Perhaps your familiarity with this field made you assume that we all knew that the diffusion treatment would be limited in depth.
Comment: @Trunk I have edited the question for completeness. The answer by rMoishe Pippik makes incomplete sense as it does not discuss any mechanisms.
Comment: @Kevin If you replace by smaller ions, the glass will not become _soft_ but very likely just brittle. Probably shatters even while you do it.

Answer 2 (26 votes):
[Chemically-strengthened glass](https://en.wikipedia.org/wiki/Chemically_strengthened_glass) is similar [tempered glass](https://en.wikipedia.org/wiki/Tempered_glass) in that the outside of the glass is under compression, while the inside is **not** compressed. If _all_ the sodium in chemically-strengthened glass were to be replaced by potassium, there would be no difference in stress between the interior and the exterior layer. How does this difference between layers help make the glass stronger? As in [prestressed concrete](https://en.wikipedia.org/wiki/Prestressed_concrete), this makes the substance stronger under tension because the initial stress counteracts that force.

Answer 3 (6 votes):
As A.K. notes, it is the substitution of larger atoms for smaller atoms that adds stress to the glass, making it stronger. So you can't increase the stress by starting with a **larger** metal, but you could on the other hand start with a **smaller** metal: [Chemically strengthened lithium aluminosilicate glass (Int. Patent Application)](https://patents.google.com/patent/WO2007032961A2/en)

Discussion on this answer:
Comment: All credit is due to A.K., I just made some minor edits


================================================================================

